UNIVERSITA’ DEGLI STUDI DI PARMA
DOTTORATO DI RICERCA IN
" SCIENZA E TECNOLOGIA DEI MATERIALI"
Printed organic electronics: towards sensing and biosensing
Prof. Enrico Dalcanale Tutore:
Dr. Salvatore Iannotta Co-Tutor:
Dr. Pasquale D’Angelo
Dottorando: Davide Vurro
This work is aimed at impacting on the sensing and monitoring of bio-signals and biomolecules relevant to assess the state of health of people possibly improving the state of the art where the available instruments generally require complex analytical methods commonly implemented by dedicated equipment in a hospital setting. Large research efforts are in progress in research labs to develop and qualify friendly usable devices that could better implement homecare and personalized monitoring aiming at intervening as early as possible to maintain the best health possible for each person.
Within this ambitious and quite challenging framework, this PhD project is contributing by developing biosensors that show quite relevant features in terms of flexibility, stretchability, conformability and biocompatibility. Features that are quite essential for devices that should be easily and efficiently interfaced with the human body. Our devices belong to the well-known family of Electrochemical Organic Transistors (OECT) and were implemented by an innovative manufacturing protocol, i.e. the Aerosol Jet Printing (AJP) technique, on flexible/stretchable biocompatible substrates.
We chose AJP technique since we believe and hence demonstrate that could be applied to a wide range of printable inks allowing the fabrication of in-line all-printed devices with high definition features.
We hence have first of all studied the printing parameters for all the needed components including contacts, active channel on different substrates, optimizing them to achieve the best definition and functionality of the materials. For the active channel we studied poly(3,4-ethylenedioxythiophene) polystyrene sulfonate (PEDOT:PSS), that could be considered the benchmark polymer in Organic Bioelectronics. We fabricated OECTs using two different flexible substrates: polyimide (Kapton) and a fibroin film. We demonstrate that we can achieve state of the art performance of our printed devices compared to similar ones in terms of architecture and materials used. For the most advanced bio- electronic sensing device, we selected fibroin film as a substrate because not only shows better biocompatibility than a Kapton foil but we could also achieve a functionality of great relevance:
optimized fibroin films give a particularly good skin self-adhesion, improving also signal transmission without the need of the commonly used gels, features that Kapton doesn’t offer without the addition of gels and other
Our OECTs printed on fibroin have hence been directly applied on the human skin for ECG signal monitoring in a standard clinical configuration.
This represents the most important achievement: the development of a fully-printed OECT on a flexible fibroin substrate that could monitor of ECG signals both in vivo and real time giving signals amplitude even better with respect to commercial electrodes with comparable time resolutions.
These results are a very good basis for the future planned activities aimed at developing devices with an increased quality response for directly monitoring bio signals generated by neuronal activity.
We have also explored skin-attachable optical sensors. To this aim, we have studied fibroin photoelastic properties that are fundamental considering the continuous mechanical stimulation induced by the human body during movement. We made experiments on the two major fibroin phases (Silk I and Silk II) by applying longitudinal strains on a silk fibroin whispering gallery mode (WGM) cavity fabricated on an optical fiber taper.
In synthesis the major relevant results shown in this thesis, concern hence materials preparation, inks development, printing optimized processes, all printed device fabrication, that have been used to develop and qualify OECTs on fibroin as very promising all printed devices for biomedical applications. We also explored fibroin itself as a base material for optical sensors, achieving the feasibility towards developing wearable optical sensor for biomedicine and rehabilitation.
We show the feasibility of fully biocompatible, cheap, easy to handle and scalable systems that could contribute to the development of wearable and all-day user electrophysiology and optical sensors. We are working to further improve the devices by increasing their sensitivity and time response mainly working on the gain and noise suppression. The idea is to possibly extend the fields of applications to neural signals, intrinsically faster and less intense than ECG, to electrophysiology, and to wearable optical sensors.
1.1 Bioelectronics ……… 1
1.2 Materials: from inorganic to organic……… . 4
1.2.1 Conductive and semiconductive Polymers ……… 5
1.2.2 PEDOT:PSS ……… 10
1.3 Organic Electrochemical Transistor (OECT)………... 14
1.3.1 OECTs performance ………. 16
1.3.2 OECT Application in bioelectronics ……… 20
18.104.22.168 OECT as Chemical and Bio-chemical sensors ………. 21
22.214.171.124 OECT as Bio-sensors ………... 22
126.96.36.199 OECTs as Bio-signal monitoring ………. 24
Chapter 22.1 Printing Technologies ………26
2.2 Screen printing techniques ……… 28
2.3 Ink-Jet printing ………. 29
2.4 Aerosol-Jet Printing ……….. 32
2.4.1 AJP Applications ……….. 38
Chapter 33.1 SILK: an ancient material of the future ………. 42
3.2 Applications of Silk Fibroin Film ……… 47
3.2.1 Fibroin as a substrate for implantable and flexible electronics ………... 47
3.2.2 Silk Fibroin as a dielectric material for electronics applications ………. 50
3.2.3 Silk Fibroin and Photonics ……….. 52
Chapter 4Materials and Methods ……… 56
4.1 Fibroin extraction: water procedure ……… 56
4.3 PEDOT:PSS ink printing characterization ……… 59
4.4 Printing on Kapton, OECT fabrication and electrical characters……….. 60
4.5 Printing OECT on Fibroin ………. 62
4.6 Monitoring ECG with direct application of OECT on the skin ………... 63
4.7 SF/PEDOT:PSS Blend Preparation ……….. 65
4.8 OECT made with the SF/PEDOT:PSS Blend and electrical characterization………... 65
4.9 Silk fibroin WGM preparation ……….. 66
4.10 WGM characterization and determination of the photoelastic properties of fibroin………. 67
Chapter 5Result and Discussion ………. 69
5.1 Printing PEDOT:PSS by Aerosol Jet technique ……….. 69
5.2 All-PDOT:PSS printed OECTs ……… 78
5.3 Organic Electrochemical Transistor (OECT) for in vivo bio-signal monitoring …………. 83
5.4 Prototyping printed OECT on Fibroin: a novel perspective for bio-signal monitoring…… 86
5.5 SF/PDOT:PSS blend for 3D OECT ………. 89
5.6 Fibroin thermal treatments………... 95
5.7 High-Q silk fibroin Whispery Gallery Microresonator ……… 96
Conclusions and Outlook………... 106
The present chapter is dedicated to the description of the most recent achievements of electronic devices as a sensor and biosensors with a particular focus on the bio signal monitoring. Section 1.1 describes the born of the bioelectronics with a particular focus on the description of the three major application fields. Section 1.2 describes the rise of the Organic Bioelectronics that presents new properties to overcome inorganic bioelectronics limits. A brief overview about the story and the working principles of organic and semiconductor polymers has been reported in Section 1.2.1.
Section 1.2.2 describes the born and the electrical properties of PEDOT:PSS, the benchmark polymer in Organic Bioelectronic; Section 1.3 reported the working principle and the properties about Organic Electrochemical Transistors (OECT) that are selected as sensors in our work. Section 1.3.1 discusses the theoretical model developed for understanding OECT working principles. Section 1.3.2 discusses the use of OECT as sensors and biosensors with a particular focus on OECT as chemical and bio- chemical sensors (Section 188.8.131.52), bio sensors (Section 184.108.40.206) and for bio signal monitoring (Section 220.127.116.11).
Bioelectronics can be defined as the study of the synergic interaction between biological systems (cells, neurons, organs, DNAs….) and electrical devices.
Luigi Galvani pioneering experiments on bioelectricity, performed in 1780 at the University of Bologna, are widely acknowledged as the starting point of the modern Bioelectronics.1 Galvani himself, introduced for the first time, the concept of “animal electricity” and hence probed the use of bioelectric forces to study living systems.
The explosion of Bioelectronics as an effective and better established research field has been taking place during the last century, when several electronic devices have been rationalized and developed determining major impacts in biology and medicine. Presently, electronic devices are commonly used in modern hospitals and represent fast developing precious tools for perspectives of healthcare. For example, defibrillators are used to save an uncountable number of lives every year, electrocardiograms (ECG) and electroencephalograms (EEG) recording represent an indispensable system for early cardiac and neuronal diseases. 3
Recent developments have been explored taking advantage of organic materials aiming at extending the range of Bioelectronics towards applications where conventional electronic devices based on
Bioelectronics and organic bioelectronics applications can be classified in three main areas (Figure 1.1):
• Drug delivery: To achieve the desired therapeutic effect limiting side effects, pharmaceutical drugs must be delivered in safety with the appropriate concentration. Safety and efficacy are the most important requirements for a drug delivery system1, and nowadays several applications are reported in pain therapy after surgery 2 and general disease treatment 3,4.
• Biosensing for chemical- and bio- markers: The possibility to functionalize electronic devices with biomarkers opens the route to biosensing applications. Biosensors are devices that combine the functionality of a bioreceptor with a transducer system to determine the amount of a biomolecule (biomarker) in a biological system and fluids. 5 According to IUPAC a biosensor was definitely as “An independent integrated receptor transducer device, which is capable of providing selective quantitative or semi-quantitative analytical information using a biological recognition element.” 6 Biosensors with several transducers and different types of bioreceptors 5 are used, for instance, in glucose detection (this is the first biosensor application) 7, enzymatic sensing and immunosensors.
• Bio-signal recording: The electrical activity of cells, tissues and organs is based on fluxes of ionic species. Ionic currents monitoring such activity is the best and most common way to determine their integrity and their functioning and Bioelectronic devices represent an ideally viable solution to analyze and measure such signals but also an effective way to stimulate specific responses and functionalities. Typical devices described in literature are Electrodes
7,8 and Thin Film Transistors (TFTs) 9,10 as well as ionic pumps.11 Depending on the specific application and the type of bio-environment, Bio-signals monitoring often requires good conformability and good biological interfaces/compatibility by the dedicated devices. The most important physical parameter to determine a good quality of signals recorded by electrodes is the impedance at the electrode interface. Electrical impedance is a measure of materials attitude at responding to the application of alternating electrical currents of various frequencies. Electrodes with a low impedance are desirable to achieve high quality bio-signals recording and a low impedance can be realized both by increasing electrode area and using low impedance materials such as, for example, poly(3,4-ethylenedioxythiophene) polystyrene sulfonate (PEDOT:PSS)12 as electrodes coatings.
Figure 1.1 Bioelectronics major devices typology
Local and site specific drug delivery as an alternative to the more classical systemic administrations.
It is a fast developing field that is based on the novel strategies boosted by the engineering of nanocarriers and nano-systems loaded with proper drugs and vehicles towards the specific site. On the other hand, biosensing, biosignaling recording and biostimulation are typically implemented by electronic devices. The miniaturization of semiconductor devices as well as the development of new classes of biocompatible materials (organic semiconductors, biopolymers5,6….) and fabrication techniques (roll to roll 7, inkjet 8,9,10, aerosol jet printing 11 ….) are opening new opportunities in biomedical and commercial applications. Organic semiconductors and polymeric substrates, combined with innovative deposition and fabrication techniques, make also possible the development of fully flexible and conformable devices. 12 Moreover, the integration of biosensors and drug delivery systems favor the device implantation and take advantage from wearability in terms of in situ diseases treatment and bio-signals recording and stimulation. 13,14
To give an indication of the evolution of the field, in Figure 1.2 the number of publications per years of bioelectronics and organic bioelectronics applications is shown. (source: Web of ScienceTM Database)
Figure 1.2: Evolution of the number of publications per year in the field of Bioelectronics.
Relevant increase is observed around the 2005. More recent is the development for organic bioelectronics. An increase in number publication in 2013 is reported.
1.2 Materials: from inorganic to organic
Materials choice plays a critical role in bioelectronics. Bio-compatibility is obviously the first requirement in order to interface electronic devices with biological systems whenever the direct contact is needed. Ideally bio-signaling rely on the ion (ionic are in-fact most of the bio-processes) to electron (our fantastic electronic world) transduction that is best made possible by materials that make simple the transduction of ionic to electronic signals.
Nonetheless, traditional inorganic devices have been the first being used in this field, even though ionic conduction is intrinsically, poor even if present at all, in inorganic crystalline conductors. The first most relevant studies in the field are based on the use of conventional electronic devices consists of the fundamental pioneering work carried out by Fromhertz. In particular, in 1991 he reported the first silicon field effect transistor (FET) coupled with neuron.13 In this study, a neuron is being successfully supported in close contact with the insulating layer of a the gate electrode immersed in an electrolyte. By applying the needed polarization voltage between the source and drain the current driven in the transistor channel resulted to be modulated by the neuron-Si interaction so that, under
microelectrodes stimulation, its activity could be directly monitored. This fundamental work has then given rise to a blossoming literature on neuron dynamics studies.
One of the main goals of the current research is to achieve efficient and sensitive in vivo recordings of bioactivity in order to study bio-functionalities and hence diagnose diseases at their early stage. To this end, on one hand, to minimize stresses and interferences with the bio-system under study, conformable and flexible devices are desirable. The biological world is a “soft world” and the Young Modulus of silicon is six orders of magnitude higher with respect to bio-materials (around 100 GPa, while the skin, for example, shows a modulus around 13 MPa 14). On the other hand, ionic conductors represent the natural interface to communicate with living beings.
To overcome these critical issues, several research groups worked to develop innovative and alternative materials. Organic insulators and semiconductors have proven to fulfill to the above requirements. Several devices based on organic materials for sensing applications are indeed reported in literature.15–17 Organic materials present wonderful and useful characteristics suitable as an active material in bioelectronic devices:
• Flexibility/stretchability 18
• Mixed electronic-ionic conduction
• Easy functionalization
• Solution processability (spin casting, 3D printing)
• Mimic of biological systems with self-assembling properties
• Possibility to decorate with biomolecules to promote cells viability
• In thin-film state are transparent and allows transmission imaging
1.2.1 Conductive and semi-conductive Polymers
Conductive and semi-conductive polymers, or intrinsically conductive or semi-conductive polymers (IPCs), are organic materials able to conduct an electrical current. 19 In literature several examples of conductive polymers are reported. The most popular ICPs are reported in Fig. 1.3
Figure 1.3: Example of major conductive and semi-conductive polymers reported in literature
IPCs show a conjugated molecular structure with a sequence of single (σ-bond) and double bonds (π- bond) along the polymeric backbone. ICPs are basically composed of carbon atoms with a sp2 hybridization, composed by three σ bonds and a pz orbital. The overlap between pz adjacent orbitals create a p delocalized state along the polymeric chain. This delocalization promotes a main route for charge mobility along the polymer backbone. A double band structure, π-band and π*-band20, is achieved by increasing the number of double bonds.
The energy difference between the highest occupied molecular orbital (HOMO), i.e. the highest occupied state in π-band, and the lowest unoccupied molecular level (LUMO), i.e. the lowest unoccupied state in the π*-band, is named energy gap (Eg). Typically for organic polymers the Eg is higher (in the visible range) than that of inorganic semiconducting materials and comparable to that of dielectric materials. For this reason, for long time polymers have been considered insulating materials.
This view changed in 1977 when Shirakawa 21 (Nobel Prize for Chemistry in 2000 together with Hegeer and MacDiarmid) produced a highly conductive polyacetylene (PA) upon doping this material by exposing it to bromide and iodine vapors. The electrical conductivity was 10 order higher than that of the undoped PA monomers.
Starting from this result, a big effort has been dedicated to increase the conductivity of π-conjugated polymers. Chemical or electrochemical procedures have been found to be effective in promoting a reversible doping of conducting polymers. This kind of doping is quite different from that of inorganic materials, where doping is generally promoted by interstitial impurities, i.e. neutral atoms infiltrated into the semiconductor lattice. 22
Chemical doping is implemented by a redox reaction causing the oxidization (p-type doping) or reduction (n-type doping) of the polymer by electron acceptors or donors. 23,24 The electrochemical doping occurs by oxidation or reduction reactions assisted by an electrode causing the ions to diffuse in or out of the polymer in order to compensate for the electrical charge on the polymeric backbone.25 Chemical doping shows some limitations that have been resolved recurring to the electrochemical doping. Through the latter procedure, the doping yields are finely controlled by the voltage applied between conductive polymer and electrodes; in addition, the doping effect via the electrochemical mechanisms is generally reversible and allows achieving both p-type and n-type doping without introducing doping species via chemical reactions.
The charge injected by doping processes generate some defects localized along the polymeric chain that induce new energy levels in the electronic structure including polarons and bipolarons that are involved in the conduction mechanisms.19
ICPs can be further classified as polymers with degenerate or un-degenerate ground state.
Polyacetylene (CH)x can presented two cis and trans isomeric forms. 26 The trans-polyacetylene is a typical example of polymer with degenerate ground state, and it is characterized by two isoenergetic forms A and B as reported in Figure 1.4.
Figure 1.4: Schematic description of soliton in PA. In a) the phase A and B of the trans- polyacetylene is reported. In the energetic diagrams the two energy curves of the degenerate phase
A and B are shown. b) reports the structure of soliton that is between the phase A and B
These two levels create a defect in the electronic-lattice system that is formed at the interconnection
of the energy gap.27 This level can be full (positive soliton), empty (negative soliton) or with only one electron (neutral soliton) in the mid gap level.
Figure 1.5: Schematic of energy level in a soliton structure. The degenerate energy level is positioned in the middle of the band gap. Neutral (only one electron), positive (no electrons) and
negative solitons (energy level full of electrons) are reported
Most of conjugated polymers, for example, polythiophene (PT), do not show a degenerate ground state but two resonance structures, i.e. the aromatic and the quinoid structure. These structures do not have the same energy, being the quinoid the most energetic structure. Hence, a non-degenerate ground state is achieved. This means that a couple of energy levels are generated in this case.
Figure 1.6: Schematic of conductive Polythiophene. In a) the aromatic and chinoid phase is reported. These phases are not degenerate and in the corresponding energetic graph is shown in b).
Injection or removal of electrons by doping process generates a defect along the polymeric chain that is named polaron. Polaron is a radical- ion couple, negative or positive, confined between the quinoid and aromatic forms. In case of positive polarons, an electron is removed from the HOMO level while in case of negative polarons an electron is addicted in the LUMO level.
Figure 1.7: Schematic diagram of polarons structure in a Polythiophene. In a) the positive polaron structure is reported. In the energy diagram on the right in the figure, the energetic levels present one full level and one with only one electron. In b) the negative polaron structure is reported. For
An extra addition of charges may induce the formation of two coupled polarons, i.e. a bipolaron (Fig.1.8).
The number of polarons and bipolarons increases upon doping levels increasing. At high doping levels, new energy levels are formed in the band gap, reducing it as a consequence of the overlapping among single polaronic energy levels, promoting thus a conductivity enhancement due to electric field assisted charge carriers drift along the polymeric chain.
Figure 1.8: Schematic of a bipolaron structure. In a) the positive bipolaron is shown together with the corresponding energy levels structure on the right side. In b) the negative positive bipolaron
with the corresponding energy levels structure is reported
Doped polyacetylene was considered for a long time as the prototype most highly conductive polymer. The main challenge in the development of a technically useful and industrially viable product is intrinsic to some polyacetylenes’ properties such as its air sensitivity to the point that it loses the doping level upon exposure to air.
The first promising approach to overcome polyacetylenes’ drawbacks was to stabilize the sensitive π-electron by heteroatoms in electron-donor substituents. For the first time, it has been realized in polyaniline by incorporating both nitrogen N and sulfur S atoms in the heterocyclic conjugated
structure, which became the most promising substituents.28 The electron donating function of N and S ring atoms stabilizes, in fact, the π-conjugated system.
A new era for ICPs started when in 1982 Taurillon and Garnier 29 observed an electrical conductivity in Polythiophene. Thiophene was electropolymerized with perchlorate or tetrafluoroborate counterions, and a 10-100 S/cm conductivity was achieved. 29 The real breakthrough in IPCs world was the discovery that oxygen substituents at 3- and 4- position in the thiophene moieties are able to stabilize the doped form, thanks to their electron donating properties. This discovery disclosed the era of highly conductive, stable and processable thiophene-based polymers, among which Poly(3- hexylthiophene-2,5-diyl) (P3HT) and Poly(3,4-ethylenedioxythiophene) (PEDOT) are the most representative ones.
In particular, PEDOT is the most known π-conductive polymer, thanks to its air stability and high conductivity. PEDOT was synthetized for the first time in 1980 using a standard oxidative chemical polymerization EDOT moieties. 30
An insoluble powder with a high conductivity was accordingly obtained. Its insolubility represents a problem for the processability. A solving is adding counterions during the reaction to balance polymer charge and to achieve solubility. Several counterions have been tested (e.g. 𝑃𝑆𝑆#, 𝐶𝑙𝑂'#, 𝐵𝐹'#,𝑁𝑂+# , 𝑆𝑂'#, etc.), and their chose is limited only by their solubility and stability in reaction conditions.
Polystirensulfonic acid (PSS) is the counterions used to form an polyelectrolyte complex (PEC) with PEDOT, where PSS is the polyanion and PEDOT the polycation. 31 Water is used as solvent for PEC synthesis and a stable and industrial scale dispersion is achieved. Nowadays, aqueous PEDOT:PSS dispersion is commercialized under the commercial name of BaytronTM by Bayer AG and CleviosTM by Heareus. PEDOT: PSS is the most known stretchable conductive polymers used in electronic field.
Its combined properties including biocompatibility (FDA approved), high stability, film-forming formation, flexibility and ionic and electronic transport, PEDOT:PSS make it the most commonly used conductive polymer for several devices such as organic strain sensors 32,33, organic field effect transistors (OFETs) and especially in organic electrochemical transistors (OECTs) 34–36.
In PEDOT: PSS suspensions PSS is always in excess with respect to PEDOT, and the weight ratio of thiophene groups to sulfonic acid groups in standard PEDOT: PSS dispersions falls in the range between 1:2,5 to 1:20.
Both conventional and innovative techniques can be used to prepare PEDOT:PSS films. A PEDOT:
PSS dispersion can be deposited in principle by all common techniques for generally used for solution processable polymers, such as spin coating, spray coating, but also electrodeposition methods.
Nevertheless, other innovative printing techniques such as screen printing 37, inkjet printing 38 and aerosol jet printing 39 have been explored and studied to deposit PEDOT:PSS in its film form.
The dispersion is typically described as being composed by gel-like particles that are composed by a polyanion PSS-rich shell and a PEDOT-enriched core. In the case of uniform films, the typical structure formed has been depicted as a “pancake-like morphology”, where there is a succession of PEDOT and PSS regions. 40 For amorphous polymers and in particular for PEDOT:PSS, the conduction mechanism is commonly described in terms of charge hopping between adjacent sites (PEDOT cores) separated by thin insulating layers (PSS shells). This means that the conductivity is morphology dependent.
Pristine PEDOT:PSS films are characterized by an electrical conductivity (σ) not exceeding 1.0 Scm1;
41,42 an increase in electrical conductivity can be achieved via the secondary doping procedure, consisting of the addition of organic polar solvents to the PEDOT:PSS suspension 43,44,45, or by post processing treatments by the use of strong acids 46,47, ionic liquids 48,49 etc.
Fan et al 50 proposed a graphical model to understand the morphologies difference between the pristine PEDOT:PSS films and the treated ones. In this model, as reported in Fig. 1.9b, an amorphous configuration is used to describe the pristine PEDOT:PSS film’s composition. The amorphous configuration is constituted by PEDOT-rich grains. This configuration can be changed by the above treatments into a highly conductive one, characterized by much more ordered and wider PEDOT cores separate by thinner PSS shells (reduction of PSS amount). The ordered PEDOT chains are bonded with PSS molecules by ionic interactions
Figure 1.9: In a) schematic PEDOT:PSS chemical structure is reported. In b) the PEDOT:PSS structure transition due to doping and post-treatment procedures with PSS- removed. 50
Several secondary dopants have been reported in literature: ethylene glycol (EG) 51,52, glycerol, dimethyl sulfoxide (DMSO) 53,54, D-sorbitol 55,56 and ionic liquids 57.
In 2002 Zhang et al 58 reported a PEDOT:PSS anode adding D-sorbitol and glycerol into the polymer dispersion. An increase in conductivity by two orders of magnitude (1 to 100 Scm-1) was achieved in this case. Kim et al 59 reported the use of DMSO as secondary dopant. A 3 wt% of DMSO addition increased the cohesion among molecules in the cast film (PSS barrier thickness decreasing). 60 Post processing treatments are also used to increase conductivity. Ouyand et al 61 demonstrated an increment in electrical conductivity by immersing PEDOT:PSS film in an EG bath. The electrical conductivity was increased from 0.4 to 200 Scm-1 due to a combined effect consisting of a transition from amorphous configuration to an ordered structure and an enlargement of PEDOT cores provoking an enhancement of interchain transport into PEDOT-rich domains.
Aleshin et al 62 showed a conductivity dependence from the temperature described by the Mott’s equation, typical of a Variable Hopping Range (VHG) conduction mechanism:
s(𝑇) =s(0) ∗ exp (− 899:;<) Eq. 1.1
where s(0) is the infinite temperature and T0 =16/(kbN(Ef)x3 for a = ¼. Here x is the distance from a site where the electron wave function to decay to 1/e of its value, often referred to as the localization length and N(Ef) is the density of states. For this reason, an annealing process around 120°C for few minutes is needed after film deposition. The thermal post deposition treatment induces a rearrangement of the film with a morphology consisting of a change of PEDOT chains form quinoid to benzoic structure. A strong phase separation between insulating PSS and the PEDOT conductive regions is achieved and the PSS excess is removed.
A strong acid post treatment is the process that enhances electrical conductivity of PEDOT:PSS films.
In this procedure H+ ions are formed due to strong acid effects provoking the formation of PSSH, a neutral form upon the combination between H+ ions and PSS- molecules.
H+ + PSS- ® PSSH
Thanks to PSSH formation, a new rearrangement in these structures is achieved. The PSSH molecule confined inside the film structure was then removed by rinsing the film in pure water. 63,64
1.3 Organic electrochemical transistor (OECT)
After his discovery in the mid-1984,65 Organic electrochemical transistors (OECTs) became one of the most interesting and largely reported transistor architectures in literature, because of their versatility in terms of applications in several fields. In particular, OECTs are promising and effective candidates for creating an interface with the biological world. The low operating voltage (below 1V), its amplification of the ion-to-electron transduction combined with relevant electro-mechanical and optical properties of PEDOT:PPS, the material most used to fabricate OECTs active channels, make OECTs a well suitable device architecture for biological applications, including bio-sensing and bio- signal recording.
A typical OECT is made of an organic semiconductor film (the channel) in contact with an electrolyte (in liquid or solid state) in which an electrode, the gate electrode, is vertically immersed in or put in contact with it (the planar configuration).
The organic semiconductor film is in contact with two (metallic) electrodes, the source and drain electrodes, that define the geometry and dimensions of the polymeric channel such as reported in Fig 1.10.
Figure 1.10: Schematic of an organic electrochemical transistor (OECT) structure. In a) is reported the set up with the vertical gate electrode, while in b) the planar gate electrode set up is
OECTs operation is controlled by two voltages applied to the drain (drain voltage Vds) and gate (gate voltage Vgs) terminals, being the source terminal grounded. The drain voltage induces a current (drain current Ids) which is proportional to the density of free holes and electrons drifting in the channel. The Vgs controls the injection of ions from the electrolyte to the permeable organic channel, thus controlling the channel doping-dedoping properties (conductivity enhancement-reduction).
PEDOT:PSS represents the benchmark organic p-type semiconductor (positive charge carriers, holes) used for fabricating the OECT channel.
OECTs can operate in two modes, depletion and accumulation respectively.66 In the depletion modes, typical for PEDOT:PSS based OECTs, an hole current is registered in the channel upon application of Vds and in the absence of Vgs; this state has been defined as the ON-state (in these conditions the channel is degenerately doped). When a positive voltage is applied to the gate electrode, cations are injected from the electrolyte into the polymeric channel. In this case a decrease in current is achieved as a function of the gate voltage due to the compensation of an excess of negative charges induced by PSS on PEDOT sites (dedoping). Hence, the current reduces reaching its minimum value (Fig.1.11a); now the device is in its OFF-state.
In the accumulation mode, the device is in its OFF-state. When a negative voltage is applied to the gate, an anion injection is achieved. In this way the number of holes increases and the transition from the OFF state to the ON state is achieved (Fig.1.11b). Due to the strong swelling and porosity of the polymer, the doping process is a typical bulk process in OECTs involving the whole material, unlike the case of organic field effect transistors (OFETs) where the conductivity change is just an interfacial phenomenon. All the active volume of the channel can be hence involved during the doping-dedoping process, and in this way, it is possible to reach large current modulations with very low applied Vgs.
Figure 1.11: Schematic of depletion and accumulation mode in a typical OECT. The transfer curves for the two operation modes are also reported. In the depletion mode a positive voltage applied to the gate electrode induces a decrease in the drain current, instead in the accumulation
The classical manufacturing process used to fabricate OECT is based on the well-known optical lithographic technique 67,68 in which the pattern is transferred to the film from a mask using a photoreactive material (photoresist) that can react under exposition to the UV-light. This technique presents some limitations such as the number of steps needed, the poor compatibility with several organic materials and the limited number of substrates that can be used. The introduction of printing techniques for devices manufacturing has fully changed the fabrication paradigm.
In 1994, the first electrochemical transistor partially fabricated using printing technologies has been reported.69 Screen printing technique has been used to deposit carbon-based source and drain electrodes and dielectric on flexible substrate (PVC).
In the early of 1990 PEDOT inks are started to use for devices manufacturing. 70 Only in 2002 the first application of PEDOT:PSS print in an OECT devices is reported. 71 The sensors were fully realized by printing and coating techniques on flexible substrates such as paper and plastic foils. This is a turning point, after which the use non-conventional substrates such as fibers 72 or non planar substrates has created unprecedented opportunities for manufacturing OECT on large scale and with inline processes on flexible substrates.
1.3.1 OECTs performances
OECTs transduce small ionic signals via the application of a gate voltage into enhanced Ids currents This process is typically described by the transfer curve, where the Ids is plotted as a function of the applied Vgs. The device transconductance (gm), calculated by performing the first derivative of Ids
with respect to the gate voltage and represents the figure of merit describing the transduction efficiency. Transconductance in OECTs is mostly due to the volumetric nature of the device response.73
The high achievable transconductance makes OECT devices ideally suited for monitoring very small biological and physiological signals.
OECT operation was firstly modeled by Bernard et al74 by introducing a well-known theoretical model.
According to the functioning scheme mentioned above and generally accepted, it is assumed that ions from the electrolyte are injected into the polymeric channel generating a change in the channel current. Accordingly, the device can be considered as the composition of two circuits: one ionic and the other electronic.
The electronic circuit describes the hole current in an organic semiconductor film from the drain to the source electrode and is modeled by the Ohm’s equation:
𝐽(𝑥) = 𝑞µ𝑝(𝑥)AB(C)
AC Eq. 1.2 Where J is the current flux, q is the elementary charge, p is the hole density, µ is the holes mobility and dV(x)/dx is the electrical field.
The Bernard model describes both the steady state and the transient OECT performance. In the OECTs’ steady state the hole mobility is considered constant, while the material composing the channel is considered impurity and defect free. The geometry of the conductive channel is shown in Fig. 1.12a. The ionic circuit is described by a capacitor in series with a capacitor, describing the flow of ions in the electrolyte and the storage of ions in the channel respectively (fig 1.12b)
Figure 1.12: Geometrical sketch of the structure used in the model. In a) the semiconductor film is reported, where x=0 is the contact point and x=L is the film length. In b) the structure of ionic and
electric circuits is combined in the semiconductor film.74
The equation describing the OECT steady state is given in Eq.1.3
𝐽(𝑥) = 𝑞
AC Eq. 1.3
When Vds < 0 is applied between drain and source electrode, the Eq.1.3 can be spitted in two part and two different regimes are achieved:
𝐼AL = 𝐺 E1 −BGH#N OBBQ PH
I J 𝑉AL for 𝑉AL ≥ 𝑉ALLTU Eq. 1.4
𝐼AL = −𝐺BPHHVWX
OBI for 𝑉AL ≤ 𝑉ALLTU Eq. 1.5
Where Vdssat is the voltage applied to reach a current in saturation regimes and G is the conductance of the organic film. Vdssat is the difference between Vgs and Vp where Vp is the pinch off voltage.
G and Vp are dependent on the geometry of the channel.
] Eq. 1.6
^P Eq. 1.7
Where t, W and L are the thickness, width, length of the channel respectively. And p0 is the initial hole density, and cd is the capacitance for area unit.
Bernard model also describes the OECT transient behavior. The transient is dominated by two phenomena: the injection of cations in the channel and the removal of holes induced by the neutralization caused by the injected cations.
In a simplified condition, when a constant gate voltage is applied, the transient behavior is consistent with the steady state current. Under these assumptions, the transient behavior for a simplified OECT is reported as:
𝐼AL_𝑡, 𝑉ab = 𝐼cc_𝑉ab +
D𝐼cc81 − 𝑓ttf
g; 𝑒𝑥𝑝 8−tU
g; Eq. 1.8
where Iss (Vg) is the steady-state source-drain current at a gate voltage Vg and ΔIss = Iss(Vg=0)-Iss(Vg).
In this equation, two different time constants are introduced, τi and τe. The time constant for the ionic transport in the electrolyte τi is dominated by the solution resistance and the capacitance of the ionic double layer. In the Guy-Chapman double layer theory the capacitance is dependent on the channel length and on the ionic concentration according to the equation τi ~ L/C1/2. To increase the time response an increase of electrolyte concentration or a decrease in channel length is necessary.
The time constant for electronic transport (τe) is instead relevant for the transient response. The electronic current depends on the ratio τe/τi, defined as
tj = µmklX
no Eq. 1.9 where l is the position of the gate electrode, L is the channel length and μ is the hole mobility.
The Bernard model gives a good fit to interpret the output of an OECT device and a quantitative prediction of the transconductance gm in the form:
𝑔q = 8\
µ𝐶∗_𝑉Ur − 𝑉ab Eq. 1.10
Where, again, W, L and t are the channel width, length and thickness respectively, while μ and C*
are the charge mobility and the capacitance for unit volume of the channel, respectively. From Eq.
1.10 a dependence of gm from the channel geometry is evinced. 35,75
The channel thickness is an important parameter to adjust the optimal value of gm for sensing and bio signal recording applications. Recently, D’Angelo et al 76 not only confirmed that the transconductance value increases with the thickness t at Vds , but also demonstrated that gm is increase with the channel voltage.
In 2010 Tarabella et al 77 demonstrated a dependence of the current modulation on the materials used as gate electrodes. They used a typical PEDOT:PSS based OECT device in combination with a NaCl 0,1 M solution used as electrolyte to study the effect of Ag and Pt gate electrodes. They demonstrated an increase in the OECT response with the Ag gate electrodes with respect to Pt ones. This experiment confirmed a transition from an operating capacitive or non-Faradaic regime in the case of Pt gate electrodes, to a regime known as Faradaic in the case of Ag gate electrodes. In the non-Faradaic regime, Vgs induces a transient current in the electrolyte and a double electrical layer (EDL) is formed at the electrolyte/electrode interface. In the Faradaic regime, a redox reaction at the gate electrode promotes a higher steady-state current in the electrolyte.78 Hence, while EDL formation corresponds to an effective reduction of the applied gate voltage along the electrolyte, the onset of the Faradaic current better assists the injection of cations into the PEDOT:PSS channel, thus inducing a faster and higher current modulation in OECTs. In addition, in the Faradaic regime there is not any measurable dependence of current modulation upon changing the gate area, while in non-Faradaic regime the OECT response depends strongly on the gate surface area, as reported in Fig. 1.13.
Figure 1.13: The transfer curve for Ag gate with two different areas (3.3 mm2 and 1.6 mm2) are practically the same with an overlap of the experimental points. This phenomenon supports the hypothesis that redox reactions at the gate electrode generate a steady state source-gate current
which dominates the performance of the OECT.77
Finally, it is worth to note that the response time strongly depends on the electrolyte nature. As expected, in the case of solid electrolytes the device time response is slower with respect to that of OECTs based on liquid electrolytes.79
1.3.2 OECT Applications in bioelectronics
Since its discovery in 1984, as described in the previous sections, OECT devices have been intensively studied due to their interesting properties such as low operating voltage, good amplification, good ion to electron amplifying transduction and good interface with biological systems. The research works dealing with OECTs’ applications is presently very large and steadily increasing in particular in the fields of chemical biochemical sensing, including, more recently, quite impressive works where OECTs’ have been demonstrated to be ideally suitable for bio-signal monitoring.
18.104.22.168 OECT as Chemical sensors and Bio-chemical sensors
In 1985 Wrigthon et al 80 demonstrated that an OECT based on polyaniline (PANI) could efficiently sense redox reagents. PANI is a polymer that modified its conductivity as a function of PH values, in
fact this polymer con switch from the un-conductive to the conductive form by a change in the PH of the electrolyte solution. For this reason, the proposed device also showed a pH sensitive response in terms of current changes.
Later on, OECT with a polyaniline has been used by Dabke et al 81 for detecting metal ions such as K+, Ba+, Na+ and Ca2+. The devices are composed by a polyaniline doped by ethers, able to detect K+ ions with at a lowest concentration of 10-7 M thanks to the generation of defects in the polymeric backbone. A new perspective was open by Bergrenn et al 82 that developed an OECT with a PEDOT:PSS active layer for selective Ca2+ sensing. A Ca+-selective ionophore deposited on a polymeric membrane on the top of the PEDOT:PSS channel and was used to selectively determine Ca2+ concentration in a liquid medium. A sensitivity for concentration around 10-4 M was achieved in this case. Starting from the same concept, Mousavi et al 93 used selective membranes in OECT devices for selective sensing of K+, Ca2+ and Ag+ with lowest concentration limits around 10-4 M, 10-
4 M and 10-5 M respectively.
The great relevance of these results in the implementation of selectivity in a device that is not intrinsically selective for different ions even though other strategies were tempted. The first systematic study on implementing ion selectivity in a OECT has been reported by Lin et al.83 They analyzed PEDOT:PSS based OECTs in sensing K+, Ca2+ and Al3+ with different ionic concentrations in the electrolyte. First, a KCl 0.1 M solution and Ag/AgCl have been used as electrolyte and gate electrode, respectively. The transfer curves for the different cationic concentrations have shown a slow shift of the effective gate voltage (the gate voltage at which the PEDOT:PSS dedoping is actually effective) to lower values upon ions concentration increases.
Figure 1.14 In a) transfer curve for several KCl concentrations measured with an Ag/AgCl gate electrode. In the inset the schematic of the devices used. In b) and c) transfer curves for Pt and Au
gate electrodes are reported. No Nernstian trend is observed by the authors for Pt and Au electrodes.83
In addition, they demonstrated the dependence of ion selectivity from the type of the gate electrode used during the experiment. The observation was that the transfer curve recorded using an Ag/AgCl (Fig.1.14a) electrode shifted to lower gate voltage values upon increasing the cationic concentration following a Nernstian trend. Meanwhile, for electrodes based on noble metals (Pt and Au) (Fig.1.14b and Fig.1.14c) higher ion sensitivities have been obtained due to the interface EDL capacitance at the gate/electrolyte interface.
22.214.171.124 OECT as Bio-sensors
Detection of glucose and determination of its level in solution is the most studied and reported application of OECTs operated in sensing mode. Contractor at al 84 demonstrated the first glucose sensor based on a polyaniline channel over which they immobilized glucose oxidase. The observed dependence of the film conductivity to the glucose concentration in the electrolytic solution, hence the sensing mechanism, was attributed by the authors to the pH change in the region near the active layer due to the glucose reaction with the glucose oxidase and a 2 mM of detection limit has been achieved.
Zhu et al 85 demonstrated a simple glucose sensor based on a OECT device at neutral pH. The device was made by PEDOT:PSS and a Pt wire as active channel and gate electrode, respectively and a Phosphate buffer saline solution (PBS) has been used as electrolyte. When glucose is added to the PBS solution, the channel current decreased dramatically due to the interaction between glucose and glucose oxidase enzyme (GOx) immobilized on the active channel.
Macaya et al 86 reported an OECT glucose sensor with a limit of detection of a few micromoles, which is within the range of human level. PEDOT:PSS and a Pt wire were used as active channel and gate electrode respectively. In contrast with the previous works, the GOx was not immobilized on the polymer but dissolved together with glucose in PBS electrolyte. In this way, a direct reaction between glucose and GOx takes place into the electrolyte, resulting in improving the device limit of detection thanks to the Faradaic current generated by the H2O2 formation.
In the 2009 Shim et al87 reported a new class of glucose sensors: an all-plastic OECT on PEDOT:PSS that has been used both as active layer and as gate electrode, in this second case previously functionalized by ferrocene mediator. Ferrocene in fact can transfer electrons from the GOx to the gate electrode giving rice to. A detection below the micromolar level has been achieved with this kind of geometry.
Starting from these results, several research groups devoted efforts on the developed of full PEDOT:PSS OECTs. Among these, Gualandi et al88 reported an all-plastic PEDOT:PSS OECT for
selective dopamine sensors. The detection limit was only about 6 µM which is still higher respect to the real amount in human fluids. The milestone of this work is the presentation of a flexible and selective sensor for dopamine.
OECTs devices have been used for sensing several kinds of analytes such as DNA strands 89,90, dopamine 88, interleukin and other biomolecules associated to the arising of degenerative diseases. 76 The proven biocompatibility of PEDOT:PSS allowed the use of OECTs as cell-based biosensors. Yan et al 91 reported the first cell-based OECT biosensor. They demonstrated the possibility to grow cells on the PEDOT:PSS active layer. The sensing mechanism was attributed to the electrostatic interaction between PEDOT:PSS and the confluent cell layer. Specifically, the presence of cells on the active layer shifted the transfer curve towards more positive gate voltages, due to the negative charge on the cell surface.
The cell-based OECT is useful for in vitro monitoring of the cells growth mechanisms and to investigate the cells activity. For example, Romeo et al 92 developed a cell-based OECT biosensor for in vitro monitoring of the cellular activities, specifically to monitor death mechanisms of tumor cells under treatment with specific drugs. The OECT has been implemented in this case by a Transwell (Twell) in which the A549 human lung cancer cells are cultivated on a porous membrane and exposed to the anticancer drugs doxorubicin. Even better sensitivity for cell death monitoring, validated by a model developed ad hoc, is achieved when compared to typical biological sage (Fig 1.15).
Figure 1.15: Schematic of front and top view of an OECT combined with a Transwell support for cell activity sensing.92
The same device geometry was used by D’Angelo et al 91 for studying osmotic stress upon osmolarity
126.96.36.199 OECTs as Bio-signal recording
The combination of biocompatibility of the device polymeric channels, superior amplifying properties, low voltage of operation and the possibility to manufacture them on a flexible and conformable substrate, makes OECTs ideal for electrophysiology signal monitoring directly on the human body and organs.
Khodagholy et al 93 reported, for the first time the in vivo use of an OECT for brain activity recording.
PEDOT:PSS has been used as active material and all the essential part of the OECT are deposited on a Parylene-C substrate that conferred flexibility and conformability to the device combined with the device biocompatibility, allow its implantation on rat brain and the recording of epileptiform activities with a LOD higher respect to the commercial electrodes.
Later on, Campana et al 94 reported an OECT for monitoring electrocardiography (ECG) directly on the skin. The device has been fabricated on a flexible and resorbable substrate (PLGA) and stick to the skin with the help of an Electrolyte gel that acts as an adhesion promoter and an impedance adapter between the skin and the PEDOT:PSS channel. In this work the human body has been used as a gate electrode and the electrical potential of human body has been used to drive the gate current. The ECG monitored with the OECT has been acquired in a typical clinical configuration and has been compared with the ECG registered with a commercial Ag/AgCl electrodes showing how a comparable signal- to-noise (SNR) could be achieved.
Starting from these results, in 2015 Leleux et al reported the application of OECT devices for ECG, electrooculography (EOG) and electroencephalography (EEG) directly on skin. To register these kinds of signals, a good amplification is needed because these three bio-signal are characterized by small voltage peaks, in the range from mV to few microvolts. To overcome this problem, the authors developed a device that presented a high transconductance, amplification of devices, at zero gate voltage95 is used so that only a voltage on the channel is needed. As reported in Fig.1.16a the classical Einthoven triangle set up has been used. 96
For ECG recording, the gate electrode was connected to the body with an Ag/AgCl electrode; a second electrode was applied on the skin in the opposite position with respect to the first one and was connected to the source. A Vds of -0.6 V was applied and the signal was acquired.
The same parameters were used for EOG and EEG monitoring upon changing the electrode position.
For EOG the electrodes were applied near the eyes (Fig. 1.16b), while for EEG recording the two electrodes were applied on the head (Fig.1.16c).
Figure 1.16: In a) Einthoven triangle set up for ECG monitoring. Two devices are used and the two signals are compared. The first device registered the ECG signal between left and right arm;
the second is connected between the left arm and left leg. In b) EOG recording set up is reported and two devices are used. The first registered right and left eye movement; the second up and down
movement. In c) the EEG set up and the signal are reported.97
More recently; Khadagholy et al 98 developed a device geometry for in vivo monitoring of EEG. The proposed geometry consists of a gate electrode coplanar with respect to the source and drain electrodes position. PEDOT:PSS modified with D-sorbitol has been used as an active layer.
PEDOT:PSS doped with D-Sorbitol works as a reservoir of ions. Among the PEDOT:PSS layer and the gate electrode an ion membrane is deposited; in this way a higher transconductance device is achieved (32,30 mS) due to the PEDOT:PSS conductivity enhancement induced by D-Sorbitol doping. The device was mounted directly on the scalp and EEG signals have been registered for 1 hour.
The present chapter is dedicated to the description of the common printing techniques for flexible and wearable devices with a particular focus on advantages and disadvantages, an important role is attributed to the Aerosol Jet Printer technique with a full description about principle and state-of-the art.
Section 2.1 describes all the printing techniques reported in literature. Section 2.2 describes the working principle of the screen printed procedure and its application for sensing and biosensing.
Section 2.3 reported the working principle of the well-known ink-jet principle with its advantages and limits.
Section 2.4 depicted the innovative and prominent aerosol jet printing (AJP) with how this process can overcome the common technique limits with a focus on its applications.
2.1 Printing Technologies
Additive manufacturing and printing electronics over flexible substrates are areas of great interest since give rise to a fantastic design freedom and architectural flexibility while requiring relatively small investment and fabrication costs at least for small and easily customizable productions also in a perspective of large area flexible electronics. On the basis of the ongoing trends, these fast evolving technologies are expected to strongly impact in particular on the on flexible/bendable sensors and conformable electronics fully exploiting polymeric materials as substrates in combination with a large variety of different materials including nano systems and biomaterials. The change of paradigm is related to the advantages that printing processes represent with respect to the traditional and expensive optical lithography. These approaches typically require simpler technological process steps, efficient use of the materials with a reduced material waste, low fabrication costs, simple generation of complex patterning and architectures combined with non-planar surfaces and in some cases compatible with additive 3D and 4D processes 99,100 so that these emerging and fast growing technologies are ideally suitable for flexible and wearable device development.
The literature demonstrating the recent developments of the field is growing rapidly including developments on actuators 101,102, light emitting diodes 103,104,105, transistors 106,107 and bio-sensors 108–
110 development. The available approaches could be classified, for the sake of simplicity and with
reference in particular to flexible sensors and electronic devices, in the two major classes: contact and non-contact printing 111 (Fig.2.1).
Figure 2.1: Schematic classification of the fundamental printing techniques (Redesigned from 111)
The contact mode printings can be considered an already traditional process used since long time in devices fabrication. This family of techniques basically consists in the use of a pre-patterned mask in contact with the substrates (flexible or non-flexible) and the inks arrive on the substrate through them
112. Examples of contact printing are: the well-known and widely spread direct transfer process, 113 rot-to roll (R2R) techniques, 114 gravure printing 115 and nanoimprinting. 116
Even though all such methods are still fast evolving including new functionalities, in the last decades, increasing efforts have been devoted to the development of new printing techniques. These non- contact printing processes have become more and more appealing because of their simplicity and versatility in terms of materials and architectures, affordability, prototyping speed, high resolution, efficient use of the materials and reduced wastes easy control adjusting a few parameters and the ability to directly fabricate devices on several types of substrates.117,118,119
2.2 Screen printing techniques
Screen printing is the most matured and widespread technology for printed electronics. It is fast and versatile in comparison with the contact printing techniques. Typically, there are two screen printing setups: flatbed and rotary. 120
Figure 2.2: Schematic of screen printing major process. In a) the flat bed process is reported; the flexible substrate is on the screen printer stage, over the substrate is imposed the pre-patterned screen and thought a squeegee the ink is led to pass thought the mask. In b) the rotary set up is shown. The flexible substrate travels between two cylinders: the impression and the rotating screen.
The rotating screen is the pre-patterned mask and inside which is positioned the squeegee and the ink reservoir 111
A screen-printing set up is composed of a screen, a squeegee, a press and the substrate. In the flatbed set up the flexible substrate is positioned on the screen-printing plate and the patterning screen allows that the ink is being squeezed through the screen on the flexible substrate. The ink reproduces hence the pattern of the screen onto the flexible substrate. The flatbed set up is typically a laboratory instrument, to scale up to an industrial level a revolving set up has been developed.
In the rotary set up there are two rotating cylinders on the opposite sides of the flexible substrate, one of which is patterned with the desired design and contains the squeegee and the inks. Relatively high speed is achieved by the rotating screen in comparison with the flatbed, with a major drawback that the rotary screens are very expensive and difficult to clean.
The typical width resolutions achievable with screen printing technique range between 50 to 100 μm with a few microns in thickness.121 The technique resolution depends on several parameters: substrate surface tension, speed, ink viscosity, angle and geometry of the pattern. 122,111
Screen printing techniques have been widely used for fabricating a number of different types of sensors and electronic devices. For example, in 1997 has been reported the first plastic transistor123 fabricated with the screen printing techniques where all the essential components are printed on a plastic substrate.
Only quite recently, in 2017, organic electrochemical transistor for selective ascorbic acid sensing 37 has been reported where flatbed printing process has used to fabricate the devices on polyester film and all the OECT components where printed. A Limit of Detection (LOD) around 80 µM is achieved.
2.3 Ink-jet printing
Ink-jet printing (IJP) is widely recognized as an efficient method for direct deposition (writing) of a functional material on a substrate (flexible or non-flexible) in a predesigned pattern. The technique is characterized by a simple low-cost process, with a low waste of materials and well suited for large area fabrication. IJP is a direct writing (DW) technique where an ink, made of functional materials dissolved or suspended in organic solvents, is directly printed on a substrate through a nozzle. 117 In the literature a series of different mechanisms to actuate/control the ink-jet nozzle are reported, among which the most prominent are the thermal 124,125, piezoelectric 126,127 and electrohydrodynamic inkjet systems. 128,129
In the thermal system the actuator to generate the ink droplets exploits the thermal expansion of the ink to generate a steady ink jet.125
The piezoelectric (PZT) system consist of a PZT actuator that generates the ink jet by an acoustic wave.126 In the electrohydrodynamic system, the solution is ejected by generating an electrical field between the nozzle and the substrate that works as counter electrode. The printing is achieved typically in two different modes: continuous (CIJ) and Drop-on-Demand (DOD).130
CIJ works by continuously ejecting drops from the reservoir at a constant frequency. After the nozzle exit a shutter system can stop the printing without turning off the flow. In the DOD mode, a signal is sent to the transducer only when the drop is needed.